The handle http://hdl.handle.net/1887/46596
olds various files of this Leiden University
Title: Gold nanorod photoluminescence : applications to imaging and temperature
ter verkrijging van
de graad van Doctor aan de Universiteit Leiden, op gezag van de Rector Magnificus prof. mr. C. J. J. M. Stolker,
volgens besluit van het College voor Promoties, te verdedigen op donderdag 9 maart 2017
klokke 13:45 uur
Promotor: Prof. dr. M. A. G. J. Orrit
Promotiecomissie: Prof. dr. N. H. Dekker (TU Delft)
Prof. dr. A. F. Koenderink (FOM Institute AMOLF) Prof. dr. E. R. Eliel
Prof. dr. M. P. van Exter Dr. ir. S. J. T. van Noort Prof. dr. T. Schmidt
Keywords: Gold Nanorods, Luminescence, Imaging, Anti-Stokes, Temperature
Printed by: Gildeprint
Front & Back: Cover art design by Camila Carattino.
Copyright © 2017 by A. Carattino
Casimir PhD Series, Delft-Leiden 2017-03
An electronic version of this thesis can be found at
Behind every thesis lies a story that involves much more people than the mere author whose name is on the cover. This book is the conclusion of four years of work in the MoNOS group at the physics institute in Leiden, where I have focused on the study of single gold nanorod luminescence and its possible applications.
The project was framed within a larger collaboration with three more groups from bio-physics, biology and chemistry. The aim of the project was utilizing single gold nanorods as labels in the nucleus of cells, focusing into the study of the glucocorticoid receptor. My part in the collaboration was the understanding of the mechanisms that give rise to the luminescence of single gold nanorods, crucial for the imaging and tracking in living cells. Even if my work was not biophysical, I always kept an eye into the biological applications of my research.
A Friday afternoon idea, triggered by postdoc Saumyakhanti Khatua evolved into what now is chapter2of this booklet. He asked me if it was possible to monitor the etching process of gold by cyanide ions in single gold nanoparticles. The first trial showed already something interesting: single particles on glass were behaving completely different than in bulk suspension. More importantly, to answer the question it was clear that we needed better software to control the setup.
Ferry Kruidenberg, a bachelor student at the time, joined the group to help develop the software even further. He designed the core layout of the program and the first graphical user interface. Together we learned about version control, instrumentation and programming patterns. Simultaneously, a master student, Irina Komen, joined the group to start working on an optical tweezer. Together we managed to obtain photothermal signals from single nanoparticles that were trapped in water and glycerol. However, the final objective was to study the fluorescence enhancement of a dye in the vicinity of the rod while away from any other surface, thus preventing sticking of the molecules to the coverslip.
Even if the results on the optical tweezer didn’t fit into this thesis, while character-izing the emission from different nanoparticles an interesting phenomenon appeared: emission at higher energies than the excitation energy, the anti-Stokes emission. This emission proved to be reasonably efficient, sometimes even comparable to the Stokes-shifted counterpart. The detection of anti-Stokes luminescence was consistent between different samples and under different conditions.
Anti-Stokes luminescence opened the door to two different approaches. Firstly it was possible to exploit the emission at shorter wavelengths to suppress the background when imaging under biological conditions. Cells are known to fluoresce under laser irradiation and therefore dim emitters such as small nanoparticles are hard to distinguish from the background. After discussing with Veer Keizer, a PhD candidate in biology belonging to the same project, we embarked into the exploitation of the anti-Stokes emission for imaging. These ideas led to Chapter3and its publication in the Biophysical Journal. It
was very well received by the reviewers, one of them qualified the findings as a “very important breakthrough”.
However, there was more in the anti-Stokes emission than solely the application to imaging. If the emission depends on temperature, it can be used as a nano-thermometer. Photothermal therapy is a fertile subject that relies on locally increasing the temperature to kill specific cells. This is achieved by shining a laser onto gold nanoparticles inside or in the vicinity of those cells. However there are so far no ways of controlling the temperature of the particles. Studying the anti-Stokes emission can be a solution to a long standing problem in the medical and biological sciences.
To prove the usefulness of the method, the measurements were performed in a tem-perature variable flow cell. An air spaced objective was needed to avoid altering the temperature of the observed area, which in turn lowered the collection efficiency. At higher temperatures (around 60oC) the setup drifts several micrometers and therefore an accurate control of temperature and a proper tracking of the particles was needed.
Chapter4shows that it is indeed possible to determine the absolute temperature of single nanoparticles just by measuring their anti-Stokes spectrum. The method does not require any form ofad-hoccalibration and can be easily implemented in any confocal microscope coupled with a spectrometer. These findings can have a major impact on photothermal therapy and in material sciences, where the question of the temperature reached by the particles has been open for more than 20 years. Testing the method in real situations is the next logical step but was outside the time frame of the thesis.
With the experience built on the anti-Stokes luminescence, characterizing the scatter-ing of sscatter-ingle gold nanoparticles at different temperatures did not prove to be particularly challenging. Since the first inception of the computer software until the last version, that allowed to acquire all the data in Chapter5, almost 4 years had passed.
This work summarizes a lot of effort by a lot of people. It neglects all the failed experi-ments and frustrations. It is important to remind that failure is only a relative measure; while we learn something either of nature or of ourselves, we are being successful.
1 Introduction 1
1.1 Light Microscopy . . . 2
1.2 Gold Nanoparticles. . . 3
1.3 Luminescence from gold nanoparticles. . . 5
1.4 Applications of gold nanoparticles . . . 7
1.4.1 Tuning the resonance of gold nanoparticles . . . 7
1.4.2 Imaging through detection of anti-Stokes emission . . . 7
1.4.3 Gold nanoparticles as nano-thermometers . . . 8
1.4.4 Plasmon damping as a function of temperature . . . 9
1.5 One program to rule them all . . . 9
References. . . 10
2 Cyanide Etching 15 2.1 Introduction . . . 16
2.2 Experimental method. . . 17
2.3 Results . . . 18
2.4 Conclusions. . . 24
References. . . 25
3 Background-Free Imaging 29 3.1 Introduction . . . 30
3.2 Experimental method. . . 33
3.3 Results and discussion . . . 35
3.4 Conclusions. . . 39
References. . . 40
4 Gold nanorods as nano-thermometers 45 4.1 Introduction . . . 46
4.2 Experimental method. . . 49
4.3 Results . . . 50
4.4 Conclusions. . . 57
References. . . 58
5 Plasmon damping as a function of temperature 63 5.1 Introduction . . . 64
5.2 Experimental method. . . 66
5.3 Results . . . 67
5.4 Conclusions. . . 71
References. . . 72
6 Conclusions & Outlook 77
6.1 General conclusions . . . 77
6.2 Outlook. . . 77
6.2.1 Cyanide etching . . . 78
6.2.2 Background suppression. . . 78
6.2.3 Temperature sensing with anti-Stokes luminescence . . . 79
6.2.4 Plasmon Damping. . . 79
References. . . 80
A Cyanide Etching 83 A.1 Solution results. . . 84
A.2 SEM images. . . 85
A.3 Background spectrum . . . 86
B Bacgkround-Free Imaging 87 B.1 Setup . . . 88
B.2 Uv-Vis spectrum . . . 89
B.3 Filters. . . 90
B.4 TEM images of rods. . . 91
B.5 White light transmission . . . 91
B.6 Full scan without dye . . . 91
B.7 Full scan without dye . . . 92
B.8 Signal-to-background of several particles. . . 93
B.9 Viability test. . . 93
References. . . 94
C Gold nanorods as nano-thermometers 95 C.1 Comparing Comsol and a simple approximation for temperature calcula-tion. . . 96
C.2 Luminescence power dependence . . . 97
Curriculum Vitæ 107
Gold nanorods are ideal candidates for complementing fluorophores in labelling appli-cations. The presence of the surface plasmon resonance generates large absorption and scattering cross sections, thus making the detection of single nanoparticles possible under a light microscope. In this introduction we will review the current status of light mi-croscopy, particularly of fluorescence microscopes. We will introduce some properties of gold nanoparticles including the plasmon resonance and we will focus into the lumines-cence emission. Finally we will briefly introduce the experimental chapters of this thesis, that correspond to applications of the luminescence ranging from imaging to temperature sensing.
MICROSCOPEShave become indispensable tools in material science and biology. The first microscopes developed by Antoni Van Leeuwenhoek in the XVII century were aimed at studying fabrics; it didn’t take long however to discover that nature was hiding amazing details beyond what the bare human eye could see. The first microscope builders focused into developing better lenses in order to obtain sharper images and therefore being able to observe even smaller structures.
With the development of the wave theory of light a fundamental limitation for optical microscopes appeared: the diffraction limit. Abbe realized that no matter how good a lens is, there will always be a limit to how much it is possible to focus light. This limit is determined mainly by the wavelength of the employed light beam and by the maximum acceptance angle of the lens. Shortening the wavelength of the sources is therefore a possible strategy to increase the resolution of a microscope.
Particles with wavelengths shorter than optical wavelengths, such as electrons, opened the possibility to investigate much smaller structures. Notably in the field of virology the electron microscope provided the evidence that researchers were long looking for: the existence of particles smaller than what optical microscopes were able to resolve. Electron microscopes are a very powerful tool but they require special sample preparations that don’t allow the study of biological processesin vivo.
With a similar strategy, the resolution of optical microscopes can be increased with the use of ultraviolet sources. Some biological samples show emission of light at longer wavelengths when irradiated with UV light, nowadays simply referred to as autofluores-cence. In 1911 German physicist Oskar Heimstädt used the the emission from bacteria to build the first fluorescence microscope. The difficulties to focus enough UV light into the sample and the low efficiency in collecting the emission made him skeptical of the success of his design. He ended his work stating,
If and to what degree fluorescence microscopy will widen the possibilities of microscopic imaging only the future will show.
Fluorescence however was not a new phenomenon. It was first observed and charac-terized during the second half of the 19th century. The pioneering works of Stokes showed that some materials when irradiated with short wavelengths emit light at longer ones. Only in the 1930s did the first applications of fluorescent materials start to emerge for biological applications. Fluorophores were employed to stain biological samples, allowing to easily detect tissue components or bacteria. Oskar Heimstädt could rest assured that his invention was starting to revolutionize biology.
At the end of the XX century a major breakthrough occurred in the field of optics: the detection of a single-molecule fluorescence in 1990. Single molecules opened the door to determine material properties that would have been hidden by ensemble averaging. The first studies were performed at low temperature (few Kelvins) and gave access to properties not only of the fluorescence of molecules themselves but also of the hosting matrices, mainly polymers and crystals. Single molecules are the bridge between the diffraction limit of far field optics and the atomic scale properties of materials.
Single-molecule microscopy also changed the way imaging can be performed. If two fluorophores are separated further away than the diffraction limit, their centers can be determined with a precision that scales as≈1/pN, withN the number of recorded photons. The possibility of localizing single molecules beyond Abbe’s limit shows how useful single-molecule detection could be. For example, tracking of single molecules could be used to study diffusion with unprecedented spatial and temporal resolutions.
In relevant biological samples, however, the density of fluorophores is such that they are not further apart than the diffraction limit. In the late 1990s it was found that the fluorescence of molecules can be switched on and off by irradiating them with specific wavelengths. This led to the development of a wide variety of techniques that rely on switching on and off molecules, and therefore they can be individually localized. Post processing the information of each fluorescent molecule allows to reconstruct images with a spatial resolution an order of magnitude higher than the diffraction limit.
Molecules, however, show two phenomena known as blinking and bleaching. At room temperature it is impossible to prevent fluorophores from going to dark states, meaning that their fluorescence signal will disappear. Blinking characterizes the process by which fluorescence disappears for a comparatively short period of time. If the molecule undergoes an irreversible transition to a dark state, the process is called bleaching. Blink-ing and bleachBlink-ing put a hard limit to the experiments that can be performed with sBlink-ingle molecules, since they cannot be observed for extended periods of time. Tracking is limited to few seconds, and imaging is limited to few frames.
As single-molecule detection allowed to bridge the length mismatch between visible light and biologically relevant scales, new agents that can fill the gap between biologi-cally relevant time scales and fluorophores’ observation times are of utmost importance. In this direction different approaches were taken, including the use of scattering in-stead of fluorescence, the use of semiconductor quantum dots and of metallic nanoparticles. The latter are the focus of this thesis and of the next few sections.
Metallic nanoparticles have been utilized for a very long time. In a fortuitous way Romans dispersed gold salts into oxide mixtures that then they melted to obtain red-coloured glass; the beautiful Lycurgus cup is the only surviving complete example of an artifact made out of such glasses. Nanoparticles in the glass have preserved their optical properties for centuries and can still be admired today. In medieval times the technique was re-discovered and became common in the fabrication of red-coloured glasses for churches throughout Europe.
fully solving Maxwell’s equations. This solution is known today as Mie scattering. The original paper compared measured and calculated scattering spectra of gold nanospheres; both experiments and theory show a peak at around 550 nm. The weaker interaction with light of longer wavelengths explains the reddish color of colloidal gold nanoparticle suspensions.
The peak observed in the spectra is related to a resonance of the oscillating conduction electrons on the surface of the metal and is known as plasmon resonance. For particles much smaller than the incident wavelength, a simplification of the Mie formalism can be made by considering only the first order electrostatic approximation. In this case the polarizability of a nanosphere of volumeV is given by
where²0is the permittivity of vacuum,²(ω) is the permittivity of the metal as a function
of the incoming excitation frequencyωand²mis the permittivity of the surrounding medium. The absorption cross section can thus be calculated asσabs=kIm(α) and the
From equation1.1it is possible to see that a resonance will appear when Re(²(ω))= −2²m.
It is important to note that the energy at which this resonance appears is therefore depen-dent not only on the particle’s material properties but also on the surrounding medium’s optical constants. In the case of elongated nanoparticles, some correction factors can be introduced to the polarizability. Several computer packages[19–21] exist to calculate with a great precision absorption and extinction cross sections of arbitrary geometries and therefore it is not worth entering into the specifics of the calculations1.
It is important to point out, however, that while nanospheres have resonances that slightly change with their radius, elongated particles such as nanorods present a longitu-dinal resonance that strongly depends on their aspect ratio. The more elongated particles will have resonances with lower energies. Moreover particles with resonances to the near infrared region show a narrower resonance, making them interesting candidates for sensing applications. In biological conditions, nanoparticles with resonances towards longer wavelengths are particularly relevant because cells are typically transparent to near-infrared wavelengths.
A standard procedure to obtain gold nanoparticles is synthesis through wet chemical methods. Even in the best of cases there will be a dispersion of shapes in the sample. The differences between nanoparticles can be observed on electron micrographs, but also optically. Slightly different particles will show different resonances and this becomes more significant for elongated particles. Minute changes in shape will lead to different plasmonic resonances, that can be observed under the microscope. In a sample of such particles it is unlikely that two of them will have the exact same resonance. Dimers and clusters will therefore have a characteristic signature since more than one resonance will be observed in general.
The distribution of resonance energies has another important advantage: studying properties that depend on the resonance does not require a new synthesis nor changing
1A complete description of how to calculate the plasmon resonance with the ADDA package can be found at:
1.3.LUMINESCENCE FROM GOLD NANOPARTICLES
the sample. Once the nanoparticles are immobilized on a substrate it is possible to characterize them individually, select the ones with particular resonances and perform the rest of the experiments on them. All the chapters in this thesis show results that were gathered through the study of different particles in the same sample and under the same exact conditions: from chemical reactions in chapter2to electron phonon coupling in chapter5and anti-Stokes luminescence in chapters3and4.
Besides the geometrical factors, nanoparticles also show a broad distribution of their quantifiable properties. For example, the quantum yields of nanoparticles that are appar-ently equivalent (similar in size, same resonance energy) can differ from each other by almost an order of magnitude. In every chapter of this thesis variations from particle to particle can be observed. Chapter2shows that the etching rates can vary from particle to particle, in chapter5we have observed that the broadening rates when increasing temperature can differ from particle to particle. It means that particles differ from each other more than what an optical or scanning electron microscopes can resolve. The only way of validating the observed results is therefore through accumulating significative statistics on single-particle measurements.
UMINESCENCE FROM GOLD NANOPARTICLES
Light emission from gold and copper was first observed by Mooradian in 1969. In his work, electrons and holes in the metal were excited with visible light and the emission was observed at longer wavelengths. Strikingly, the emission quantum yield (i.e. the number of emitted photons per absorbed photon) that he estimated was in the order of 10−10. In
subsequent years several studies showed that this low number could be increased with the presence of sharp edges or tips, but still it would be much lower than the typical fluorescence yield of organic dyes, on the order of few percent at least.
When transitioning from bulk gold to nanoparticles, the interaction of light with metals will be highly influenced by the presence of the plasmon resonance. On one hand nanoparticles will have large absorption cross sections in specific wavelength regions, as explained in the previous section. On the other hand the emission spectrum will also be enhanced for frequencies around the plasmon resonance. Previous work has already shown a big overlap between the scattering and the emission spectra of gold nanoparticles.
The emission quantum yield of single gold nanoparticles is several orders of mag-nitude higher than bulk values partly due to the presence of sharp structures such as edges and tips. Typical quantum yield values are in the order of 10−6, several orders of magnitude lower than those of organic dye molecules, but the absorption cross section can be in the order of 10−2µm2, 6 orders of magnitude higher than those of dye molecules. The combination of both factors makes it possible to use luminescence to detect single gold nanoparticles in a standard fluorescence microscope.
plasmonic emission, but doesn’t fully exploit the advantage of the larger absorption cross section that the resonance provides.
The other approach to observe luminescence from nanoparticles is to excite them close to their resonances. In this way it is possible to benefit from the higher absorption cross section leading to lower excitation powers. Recent studies have shown that the emission quantum yield does not change significantly between exciting at the resonance and exciting with a shorter wavelength around 532 nm. However, the photolumines-cence itself is also coupled to the plasmon; if excited in resonance, the emission will be concentrated around the excitation wavelength. Detection filters may therefore block an important part of the emission spectrum.
Throughout this thesis luminescence will refer to all the emission from a nanoparticle at different wavelengths than the excitation wavelength and that scales linearly with the excitation power. Luminescence makes it is possible to observe single gold nanoparticles under a conventional fluorescence microscope. A notch or long pass filter in the detection path efficiently blocks the excitation light while allowing the luminescence emission to go through. Moreover it is possible to select nanoparticles with resonances at wavelengths at which no other sources absorb or emit, effectively lowering the background.
For dye molecules the Stokes shifted fluorescence can be understood as a consequence of energy conservation: a photon of a given energy excites the electrons of a material that subsequently relax back by emitting another photon, by transferring energy in the form of heat to the medium or a combination of both. It is expected therefore that the emitted photon has a lower energy than the incident one. This is always valid unless the excited electrons can somehow gain energy from the medium before relaxing back radiatively. If this happens, the process is called anti-Stokes and the emitted photons possess a higher energy than the excitation.
When excited at resonance, gold nanoparticles exhibit anti-Stokes luminescence with intensities that can be compared to the Stokes shifted emission. In brief, the mechanism proposed for the emission of photons with higher energies is the interaction of electrons and holes with phonons in the gold lattice before they recombine radiatively. Note that in this process the interaction with other thermal charge carriers is also possible. Assuming that the anti-Stokes emission from gold nanoparticles depends only on the population of phonons, the general shape of the emission is expected to be
kBT − 1
whereωis the frequency of the emitted photon,kBis Boltzmann constant andT is the temperature.
1.4.APPLICATIONS OF GOLD NANOPARTICLES
PPLICATIONS OF GOLD NANOPARTICLES
TUNING THE RESONANCE OF GOLD NANOPARTICLES
The previous two sections highlighted different strategies for detecting single gold nanopar-ticles such as nanospheres or nanorods. The principal characteristic of the parnanopar-ticles is their localized surface plasmon resonance. The resonance wavelength (or energy) will be given by the geometry of the particle and by the surrounding medium’s properties, such as its refractive index. The geometry of the particles is determined during the synthesis procedure, where the average length and width can be tuned. However, when the particles are deposited on a substrate, their resonance is already determined.
Chapter2focuses into tuning the plasmon resonancein-situ, once they are immo-bilized on a substrate and optically characterized. Currently two approaches exist for tuning the plasmon resonance after synthesis: (1) it is possible to tune the refractive index of the medium using an electric or magnetic field. (2) It is possible to induce shape modifications of the nanoparticles either through chemical[34–38] or physical means[25,39,40]. In the majority of the reports a blue shift of the plasmon resonance has been observed.
In the case of chemical etching of the nanoparticles, almost all works have focused on bulk measurements in suspension. The tips of the particles tend to be more reactive because they are less protected by the surfactants that prevent aggregation of particles. This leads to an anisotropic reaction that slowly transforms elongated particles into spheres and that softens sharp edges or tips, yielding an overall blue-shift of the resonance. Chapter2shows that through well known chemistry between gold and cyanide ions it is possible to induce a red-shift of the plasmon. This is modelled through an isotropic etching of the particles, and a good agreement between calculations and experiments is obtained. The main difference with previous work is the absence of a capping agent on the particles’ surface. Controllably changing the shape of nanoparticles is of great importance for experiments where a specific resonance is needed.
IMAGING THROUGH DETECTION OF ANTI
Gold nanoparticles are ideal candidates for labelling biological samples because they prove to be innocuous to the cell but also because they can be observed for extended periods of time[28,42]. One of the drawbacks of gold nanoparticles is their low quantum yield. Since the absorption cross section of the particles scales as their volume, detecting smaller particles in presence of background requires a specific approach.
To overcome these difficulties, several techniques have been developed for imag-ing gold nanoparticles, includimag-ing two-photon excited luminescence, photothermal heterodyne detection and interferometric detection. Each of these methods is useful but their operation requires dedicated setups and a high level of expertise.
nanoparticle through conventional Stokes-shifted emission while the anti-Stokes scheme presents a signal-to-background ratio higher than 10.
The technique presented in chapter3can be readily implemented in any conventional microscope by the addition of the appropriate filters. It does not require any special operation nor infrastructure. Moreover any data analysis tool for tracking, imaging, centroid extraction, etc. of single labels can readily be implemented without further modifications.
GOLD NANOPARTICLES AS NANO
Figure 1.1: Number of papers published containing the terms Plasmonic Photo Thermal Therapy since 1995. Note the logarithmic scale in the y-axis.
During the past two decades there has been an increasing interest in gold nanoparti-cles as possible agents for medical treatments[46–48]. The strong interaction between particles and light makes them ideal candidates not only for labelling but also for releasing heat into very localized environments [46,47,49,50]. This simple approach can be used for instance to induce death of cancer cells and is normally referred to as Plasmonic Photo Thermal Therapy (PPTT or PTT depending on the author). Figure1.1shows the number of papers published in this field since 1995. The increase in the number of publications is more than exponential, and depicts the relevance this technique is gaining over time.
After decades of research there is however almost no information regarding the tem-peratures that need to be reached by the nanoparticles to induce cell death. Much less is available at a single-particle/single-cell level. Moreover the field of thermometry at the nanoscale is subject to a heated debate[51,52] since some experimental findings contradict expected values from thermodynamic considerations.
Chapter4of this thesis focuses into the characterization of the mechanisms that give rise to anti-Stokes luminescence. Discarding multi-photon processes, photons with higher energies than the excitation energy require interactions with thermal baths. In a nanoparticle electrons and holes can interact with phonons before recombining radiatively, as discussed in section1.3.
1.5.ONE PROGRAM TO RULE THEM ALL
shows the changes that the luminescence spectra undergo when increasing the medium’s temperature.
The calibration-free procedure is a major improvement over previous techniques in the field of nano-thermometry. The results from the chapter can have a significant impact on an emerging community that addresses one of the most pressing health issues of our time.
PL ASMON DAMPING AS A FUNCTION OF TEMPERATURE
Luminescence is not the only method for detecting gold nanorods with an optical mi-croscope. Gold nanoparticles have a large scattering cross section coinciding with the plasmon resonance. Exciting nanoparticles with white light allows one to record the scattering spectra in any confocal microscope coupled to a spectrometer. Since the reso-nance itself is affected by the surrounding conditions[54,55], it is possible for example to use it for studying changes in the refractive index of the medium. However the plasmon resonance energy is not the only interesting property of the nanoparticles; the plasmon damping rate can also be used to detect changes in the surrounding conditions.
In principle there are four main mechanisms responsible for damping of the plasmons[22,56,57]: phonon coupling, surface interactions, electron-electron collisions and radiative damping. Out of those only the coupling with phonons shows an appreciable dependence on temperature[54,55]. Therefore studying the depen-dence of the plasmon width with temperature could lead to an alternative approach to measure temperature changes.
Chapter5focuses on the characterization of the plasmon resonance of single gold nanorods at various temperatures. In the range of temperatures studied (between 293 K and 350 K), the plasmon width increases linearly with temperature. The broadening is assigned to an increase in the electron-phonon damping rate, and the observations can be understood through the Debye model of phonons. Measuring the broadening of the resonance can then be related to changes in temperature of the surrounding medium.
The scattering of gold nanorods is much more efficient than their luminescence, not only because of their large scattering cross section but also because of the low quantum yield of their emission. Therefore the powers needed for recording scattering spectra are much lower than the ones employed when exciting the luminescence of the parti-cles. These lower powers enable studies of the plasmon resonance without inducing a significative increase of temperature. However the broad distribution of widths and broadening rates found in the studies of chapter5does not allow to perform an absolute temperature measurement but only to measure a relative change. This is similar to other experiments performed with quantum dots and therefore expands the toolbox of available techniques for thermometry at the nanoscale.
NE PROGRAM TO RULE THEM ALL
on the fly. Experiments performed at CERN and in other particle physics accelerators heavily rely on computers to discard millions of non-interesting events and save the relevant ones. However, for the average experimentalist there is a big gap between what is needed and what is available.
Flexible, open source programs to control experiments are hard to find in the Internet if they exist at all. The absence of a solution generates a double negative effect: researchers find themselves reinventing the wheel more often than desired and experiments are based on what can be done and not on what is desired to be done. For example, a simple home-built confocal microscope requires a dedicated computer program to run, which can take months to develop. Commercial software normally lacks the flexibility that new science needs, limiting the creativity of researchers while planning experiments.
All the chapters of this thesis relied on a flexible computer program that allowed to plan complex experiments building on software rather than being limited by it. The program has been made open source and can be found on Github2. It started to be developed for simplifying repetitive tasks such as refocusing on a particle or triggering a spectrometer. Later it evolved into a fully functional graphical user interface (GUI) for performing and visualizing 2D and 3D scans, acquiring fast timetraces, monitoring an optical tweezer and communicating with serial devices as well as over the network. The latest developments of the software open the possibility to define an application programming interface (API) for easy integration with applications on smartphones or to control several independent setups through the local network or also through the Internet.
Chapter2shows results where several particles were analyzed while being etched with potassium cyanide. Studying several nanoparticles under the same conditions is crucial for characterizing the dependence with the plasmon resonance and to discard any systematic error. Refocusing on the particles by hand is too slow for processes that happen as fast as the ones shown in the chapter and therefore the experiments wouldn’t have been possible without a specialized computer program.
Chapter3shows the scanning capabilities of the software for imaging purposes. Moreover the specific program for acquiring the power dependence plots can be written in about 20 lines of code. When varying the temperature of the sample as done in chapters
4and5, being able to refocus on a reference particle to compensate for the drift of the setup was of utmost importance.
The software even if developed with an optical microscope in mind, can be easily ex-tended to other configurations. Choosing Python as the programming language provides platform independence; it can run without inconvenience on several Windows versions, Mac OS and Linux. The main objective of the program is to provide a lower level layer on which to build creative solutions to complex problems.
 G. A. Kausche, E. Pfankuch, and H. Ruska,Die Sichtbarmachung von pflanzlichem Virus im ubermikroskop,Naturwissenschaften27, 292 (1939).
 O. Heimstädt,Das Fluoreszenzmikroskop,Z. Wiss. Mikrosk.28, 330 (1911).
 N. Rusk,Milestones in light microsopy: The fluorescence microscope,Nature (2009), 10.1038/ncb1941.
 J. S. Ploem,The use of a vertical illuminator with interchangeable dichroic mirrors for fluorescence microscopy with incident light,Z. Wiss. Mikrosk.68, 129 (1967).
 M. Orrit and J. Bernard,Single pentacene molecules detected by fluorescence excitation in a p -terphenyl crystal,Phys. Rev. Lett.65, 2716 (1990).
 T. Schmidt, G. J. Schutz, W. Baumgartner, H. J. Gruber, and H. Schindler,Imaging of single molecule diffusion.Proc. Natl. Acad. Sci.93, 2926 (1996).
 W. E. Moerner, R. M. Dickson, A. B. Cubitt, and R. Y. Tsien,On/off blinking and switching behaviour of single molecules of green fluorescent protein,Nature388, 355 (1997).
 E. Betzig, G. H. Patterson, R. Sougrat, O. W. Lindwasser, S. Olenych, J. S. Bonifa-cino, M. W. Davidson, J. Lippincott-Schwartz, and H. F. Hess,Imaging Intracellular Fluorescent Proteins at Nanometer Resolution,Science (80-. ).313, 1642 (2006).
 T. Dertinger, R. Colyer, G. Iyer, S. Weiss, and J. Enderlein,Fast, background-free, 3D super-resolution optical fluctuation imaging (SOFI),Proc. Natl. Acad. Sci.106, 22287 (2009).
 W. E. Moerner,New directions in single-molecule imaging and analysis,Proc. Natl. Acad. Sci.104, 12596 (2007).
 M. Orrit,Chemical and physical aspects of charge transfer in the fluorescence inter-mittency of single molecules and quantum dots,Photochem. Photobiol. Sci.9, 637 (2010).
 R. Zondervan, F. Kulzer, M. A. Kol’chenk, and M. Orrit,Photobleaching of Rhodamine 6G in Poly(vinyl alcohol) at the Ensemble and Single-Molecule Levels,J. Phys. Chem. A108, 1657 (2004).
 J. Ortega-Arroyo and P. Kukura,Interferometric scattering microscopy (iSCAT): new frontiers in ultrafast and ultrasensitive optical microscopy,Phys. Chem. Chem. Phys. 14, 15625 (2012).
 A. P. Alivisatos, W. Gu, and C. Larabell,Quantum dots as cellular probes,Annu. Rev. Biomed. Eng.7, 55 (2005).
 X. Huang, S. Neretina, and M. A. El-Sayed,Gold nanorods: from synthesis and properties to biological and biomedical applications,Adv. Mater.21, 4880 (2009).
 D. J. Barber and I. C. Freestone,An investigation of the origin of the colour of the Lycurgus Cup by analytical transmission electron microscopy,Archaeometry32, 33 (1990).
 C. F. Bohren and D. R. Huffman,Absorption and scattering of light by small particles
(John Wiley & Sons, 2008).
 M. A. Yurkin and A. G. Hoekstra,The discrete-dipole-approximation code ADDA: Capabilities and known limitations,J. Quant. Spectrosc. Radiat. Transf.112, 2234 (2011).
 A. F. Oskooi, D. Roundy, M. Ibanescu, P. Bermel, J. D. Joannopoulos, and S. G. Johnson,MEEP: A flexible free-software package for electromagnetic simulations by the FDTD method,Comput. Phys. Commun.181, 687 (2010).
 B. T. Draine and P. J. Flatau,Discrete-Dipole Approximation For Scattering Calcula-tions,J. Opt. Soc. Am. A11, 1491 (1994).
 C. Sönnichsen, T. Franzl, T. Wilk, G. von Plessen, J. Feldmann, O. Wilson, and P. Mulvaney,Drastic Reduction of Plasmon Damping in Gold Nanorods,Phys. Rev. Lett.88, 077402 (2002).
 L. Vigderman, B. P. Khanal, and E. R. Zubarev,Functional gold nanorods: Synthesis, self-assembly, and sensing applications,Adv. Mater.24, 4811 (2012).
 K. Lindfors, T. Kalkbrenner, P. Stoller, and V. Sandoghdar,Detection and Spectroscopy of Gold Nanoparticles Using Supercontinuum White Light Confocal Microscopy,Phys. Rev. Lett.93, 037401 (2004).
 M. Yorulmaz, S. Khatua, P. Zijlstra, A. Gaiduk, and M. Orrit,Luminescence quantum yield of single gold nanorods.Nano Lett.12, 4385 (2012).
 A. Mooradian,Photoluminescence of metals,Phys. Rev. Lett.22, 185 (1969).
 G. T. Boyd, Z. H. Yu, and Y. R. Shen,Photoinduced luminescence from the noble metals and its enhancement on roughened surfaces,Phys. Rev. B33, 7923 (1986).
 M. B. Mohamed, V. Volkov, S. Link, and M. A. El-Sayed,The ‘lightning’ gold nanorods: fluorescence enhancement of over a million compared to the gold metal,Chem. Phys. Lett.317, 517 (2000).
 E. Dulkeith, T. Niedereichholz, T. Klar, J. Feldmann, G. von Plessen, D. Gittins, K. Mayya, and F. Caruso,Plasmon emission in photoexcited gold nanoparticles,
Phys. Rev. B70, 205424 (2004).
 M. Beversluis, A. Bouhelier, and L. Novotny,Continuum generation from single gold nanostructures through near-field mediated intraband transitions,Phys. Rev. B68, 1 (2003).
 R. Sundararaman, P. Narang, A. S. Jermyn, W. a. Goddard III, and H. a. Atwater,
Theoretical predictions for hot-carrier generation from surface plasmon decay,Nat. Commun.5, 5788 (2014).
 P. A. Kossyrev, A. Yin, S. G. Cloutier, D. a. Cardimona, D. Huang, P. M. Alsing, and J. M. Xu,Electric field tuning of plasmonic response of nanodot array in liquid crystal matrix,Nano Lett.5, 1978 (2005).
 N. R. Jana, L. Gearheart, S. O. Obare, and C. J. Murphy,Anisotropic Chemical Reac-tivity of Gold Spheroids and Nanorods,Langmuir18, 922 (2002).
 J. Rodríguez-Fernández, J. Pérez-Juste, P. Mulvaney, and L. M. Liz-Marzán, Spatially-directed oxidation of gold nanoparticles by Au(III)-CTAB complexes.J. Phys. Chem. B
109, 14257 (2005).
 E. Carbó-Argibay, B. Rodríguez-González, J. Pacifico, I. Pastoriza-Santos, J. Pérez-Juste, and L. Liz-Marzán,Chemical Sharpening of Gold Nanorods: The Rod-to-Octahedron Transition,Angew. Chemie119, 9141 (2007).
 C. K. Tsung, X. Kou, Q. Shi, J. Zhang, M. H. Yeung, J. Wang, and G. D. Stucky,Selective shortening of single-crystalline gold nanorods by mild oxidation,J. Am. Chem. Soc.
128, 5352 (2006).
 W. Ni, X. Kou, Z. Yang, and J. Wang,Tailoring longitudinal surface plasmon wave-lengths, scattering and absorption cross sections of gold nanorods,ACS Nano2, 677 (2008).
 S. Link, C. Burda, B. Nikoobakht, and M. A. El-Sayed,Laser-Induced Shape Changes of Colloidal Gold Nanorods Using Femtosecond and Nanosecond Laser Pulses,J. Phys. Chem. B104, 6152 (2000).
 Y. Horiguchi, K. Honda, Y. Kato, N. Nakashima, and Y. Niidome,Photothermal reshaping of gold nanorods depends on the passivating layers of the nanorod surfaces,
Langmuir24, 12026 (2008).
 N. Lewinski, V. Colvin, and R. Drezek,Cytotoxicity of nanopartides,Small4, 26 (2008).
 J. Pérez-Juste, I. Pastoriza-Santos, L. M. Liz-Marzán, P. Mulvaney, J. Perezjuste, I. Pas-torizasantos, L. Lizmarzan, and P. Mulvaney,Gold nanorods: Synthesis, characteriza-tion and applicacharacteriza-tions,Coord. Chem. Rev.249, 1870 (2005).
 B. van den Broek, B. Ashcroft, T. H. Oosterkamp, and J. van Noort,Parallel Nano-metric 3D Tracking of Intracellular Gold Nanorods Using Multifocal Two-Photon Microscopy,Nano Lett.13, 980 (2013).
 S. Berciaud, D. Lasne, G. Blab, L. Cognet, and B. Lounis,Photothermal heterodyne imaging of individual metallic nanoparticles: Theory versus experiment,Phys. Rev. B
 F. Ignatovich and L. Novotny,Real-Time and Background-Free Detection of Nanoscale Particles,Phys. Rev. Lett.96, 013901 (2006).
 A. M. Gobin, M. H. Lee, N. J. Halas, W. D. James, R. A. Drezek, J. L. West, M. Gobin, M. H. Lee, N. J. Halas, W. D. James, R. A. Drezek, and J. L. West,Near-Infrared Reso-nant Nanoshells for Combined Optical Imaging and Photothermal Cancer Therapy,
Nano Lett.7, 1929 (2007).
 X. H. Huang, I. H. El-Sayed, W. Qian, and M. a. El-Sayed,Cancer cell imaging and photothermal therapy in the near-infrared region by using gold nanorods,J. Am. Chem. Soc.128, 2115 (2006).
 S. Huo, S. Jin, X. Ma, X. Xue, K. Yang, A. Kumar, P. C. Wang, J. Zhang, Z. Hu, and X.-J. Liang,Ultrasmall Gold Nanoparticles as Carriers for Nucleus-Based Gene Therapy Due to Size-Dependent Nuclear Entry,ACS Nano8, 5852 (2014).
 X. Huang, P. K. Jain, I. H. El-Sayed, and M. A. El-Sayed,Plasmonic photothermal therapy (PPTT) using gold nanoparticles,Lasers Med. Sci.23, 217 (2008).
 L. R. Hirsch, R. J. Stafford, J. A. Bankson, S. R. Sershen, B. Rivera, R. E. Price, J. D. Hazle, N. J. Halas, and J. L. West,Nanoshell-mediated near-infrared thermal therapy of tumors under magnetic resonance guidance.Proc. Natl. Acad. Sci. U. S. A.100, 13549 (2003),arXiv:0008204 [cond-mat].
 J.-M. Yang, H. Yang, and L. Lin,Quantum Dot Nano Thermometers Reveal Heteroge-neous Local Thermogenesis in Living Cells,ACS Nano5, 5067 (2011).
 M. Suzuki, V. Zeeb, S. Arai, K. Oyama, and S. Ishiwata,The 10ˆ5 gap issue between calculation and measurement in single-cell thermometry, Nat. Methods12, 802 (2015).
 M. K. Sato, M. Toda, N. Inomata, H. Maruyama, Y. Okamatsu-Ogura, F. Arai, T. Ono, A. Ishijima, and Y. Inoue,Temperature Changes in Brown Adipocytes Detected with a Bimaterial Microcantilever,Biophys. J.106, 2458 (2014).
 M. Liu, M. Pelton, and P. Guyot-Sionnest,Reduced damping of surface plasmons at low temperatures,Phys. Rev. B79, 035418 (2009).
 A. Konrad, F. Wackenhut, M. Hussels, A. J. Meixner, and M. Brecht,Temperature Dependent Luminescence and Dephasing of Gold Nanorods,J. Phys. Chem. C117, 21476 (2013).
 C. Novo, D. Gomez, J. Perez-Juste, Z. Zhang, H. Petrova, M. Reismann, P. Mulvaney, and G. V. Hartland,Contributions from radiation damping and surface scattering to the linewidth of the longitudinal plasmon band of gold nanorods: a single particle study,Phys. Chem. Chem. Phys.8, 3540 (2006).
TUNING OF GOLD NANOROD
PL ASMON THROUGH OXIDATIVE
Single gold nanorods exhibit great opportunities for bio-sensing, enhanced spectroscopies and photothermal therapy. A key property of these particles is the surface plasmon reso-nance, that is strongly dependent on their shape. Methods for tuning this resonance after the synthesis of the particles are of great interest for many applications. In this work we show that, through very well known chemistry between gold atoms and cyanide ions, it is possible to tune the surface plasmon of single25×50nm rods by more than100nm towards longer wavelengths. This is achieved by slowly etching gold atoms from the surface of the particles, preserving their specific optical properties.
This chapter has been published in Physical Chemistry Chemical Physics 18, 15619-15624 (2016).
GOLDnanoparticles exhibit large absorption and scattering cross sections with reso-nances ranging from the visible to the near-infrared. This property is closely related to the surface plasmon, a collective oscillation of conduction electrons that depends on the shape of the particles. For gold nanorods (AuNR) the surface plasmon resonance (SPR) wavelength depends on the aspect ratio (AR) of the particle and can be found between 540 nm for spheres with AR of 1 to beyond 800 nm for elongated particles. The SPR of gold particles can be observed by recording their scattering or luminescence spectrum. Both show a near exact overlap for a large range of wavelengths.
The surface plasmon presents great opportunities in (bio-) sensing, enhanced spec-troscopies , photothermal therapy and for concentrating light below the diffraction limit. Success in many of these applications requires precise andin situcontrol over the nanoparticles’ plasmon resonance energy. For example, maximum fluorescence or Raman enhancement is achieved when the nanoparticles’ plasmon resonance is tuned to the excitation laser wavelength. As another example, efficient photothermal therapy requires the nanoparticles’ SPR to be tuned to the near-IR to minimize the damage to healthy cells.
Typically the SPR is tuned by carefully manipulating the shapes of nanoparticles during their synthesis. Particularly useful are the rod-shaped particles, whose resonance can be found between 600 nm and beyond 1000 nm, depending on their aspect ratios. Adjusting the concentrations of gold seeds and silver nitrate during the seed-mediated growth is the usual way for producing particles with different resonances. Many other nanoparticle shapes such as nanoprisms, nanorice, nanocubes, nanoshells, etc. have been synthesized with their plasmon resonances covering the entire spectral range from visible to near-IR. Wet-chemical synthesis methods, however, generally yield a broad distribution in nanoparticle sizes and/or shapes, hindering precise and reproducible experiments that need a particular resonance. Furthermore, these methods do not provide anyin situadjustment of the SPR, any change of which requires a new synthesis.
For the past decade, single-particle experiments have provided insight into processes that would have been averaged out in bulk experiments. For instance, pump and probe experiments on single particles avoid assumptions regarding size distributions of the sample[12,13]. Nonlinear processes such as second (or third) harmonic generation can be studied when the particles’ plasmon is well characterized and single-particle experiments allow to overcome the inhomogeneous broadening of a sample in suspension[14,15]. Enhanced spectroscopies normally rely on well defined structures fixed on a substrate. Most of these experiments will benefit from techniques that allow to tunein situthe plasmon resonance and geometry of specific particles once they are immobilized on a substrate and optically characterized.
Figure 2.1: Experimental setup and examples of observations. a) Simplified schematic of the confocal micro-scope employed during the measurements. b) A typical 1-photon luminescence raster scan of the sample immersed in water, before etching and c) luminescence spectrum of a single rod.
or physical means. For example, thermal reshaping was induced by illuminating the nanoparticles with an intense, pulsed [18,19] or continuous laser. Increasing the particles’ temperature therefore leads to changes in shape, favoring those conformations with a lower surface energy (i.e. spheres over rods, etc.). Chemical reshaping is also possible and was the focus of several studies[20–24]. In those cases, the capping agent will induce different reactivities on the sides than on the tips of the particles; because of a higher curvature the tips are normally more susceptible to chemical reactions, leading to an anisotropic reshaping shortening the long axis or softening any high-curvature region. Both in the case of laser-induced or chemical-induced reshaping the outcome is usually a blue-shift of the surface resonance peak.
In this work we present a new approach for precise andin situtuning of plasmon res-onances of single gold nanorods isolated and immobilized on a glass surface. A nanorod’s plasmon resonance is tuned over 130 nm, starting from 650 nm up to 780 nm. Our method exploits well-known chemistry between gold and cyanide ions (CN−) to controllably etch gold atoms from the nanoparticle and thereby change its aspect ratio. We note that unlike many of the previous studies, here we observe a SPR red shift on gold nanorods. We also verified the resuts from scanning electron microscopy (SEM) images of the particles and by simulations based on the discrete dipole approximation method. Contrary to previous works where the etching was preferred at the tips, we attribute the red shift to isotropic etching of gold nanorods from all sides resulting in an increase of aspect ratio.
Single-particle measurements were done on a home-built confocal microscope (Fig-ure2.1a). A 532 nm laser was used for exciting the particles. The excitation power was 300µW at the back aperture of the objective (Olympus 60×, NA 0.9 air). Since the laser employed is not in resonance with the longitudinal plasmon, the power dissipated by the particles is not high enough as for showing thermal reshaping. After several minutes of ir-radiation the plasmon position didn’t show any shift. Typical powers needed for reshaping are in the range 1−5 mW. The luminescence signal was filtered with two 532 nm notch filters and was detected by either an avalanche photodiode or a liquid-nitrogen-cooled CCD-spectrometer (Acton 500i). The images were acquired by scanning the sample across the tightly focused laser beam using a XYZ piezo scanning stage (PI Nano Cube). Figure
2.1b shows a typical result from a raster scan. Each bright spot corresponds to a single nanoparticle.
Samples were prepared by spin-casting a suspension of AuNR on clean coverslips. Afterwards the slides were thoroughly rinsed with Milli-Q water and placed in an ozone cleaner for one hour to eliminate any trace of the surfactant (cetyltrimethylammonium bromide, CTAB.) To perform the measurements, the samples were mounted on a flowcell and the initial spectra were taken with the rods immersed in Milli-Q water. Figure2.1c shows an example of the luminescence spectrum of a single particle. Having this initial characterization allowed us to discard clusters of rods from the study.
Of each sample, approximately 10 different particles were selected. Afterwards a solution of KCN was flowed into the sample chamber and spectra of each particle were acquired consecutively after focusing on each one. The time resolution varies according to the exposure time and number of particles studied; in this work a spectrum of each particle was taken at least every minute. Concentrations of KCN ranging from 10µM to 80µM were employed with different samples.
Figure2.1b shows a typical one-photon-excited luminescence image of gold nanorods isolated on a glass surface and covered with water. Single-particle spectra display a narrow Lorentzian lineshape while clusters show additional features or a broad spectrum. Figure2.1c shows a typical spectrum originating from a single nanoparticle. In the samples analyzed more than 90% of the diffraction-limited bright spots originate from single gold nanorods.
Figure2.2shows the one-photon luminescence spectra of a gold nanorod immersed in 20µM KCN at intervals of 70 s. We clearly observe a gradual red shift of the nanorod’s plasmon resonance by more than 100 nm over a time interval of 300 s. The left inset of Fig.2.2shows the integrated intensity of the particle as a function of time. It is possible to observe a decrease of the intensity by a factor 4 during the same interval in which the shift was observed. Fitting each spectrum with a Lorentzian function allows to extract the resonance wavelength at each recorded time. A more detailed analysis shows that the nanorod’s plasmon resonance wavelength varies almost linearly with time as shown in the right inset of Fig.2.2a
Figure 2.2: One-photon-excited luminescence spectra of gold nanorods immersed in 20µM KCN. The different curves show the plasmon shift of a single rod. Each shown spectrum was acquired at 70 s intervals. The insets display the integrated intensity of the peak and the resonance wavelength as functions of time, respectively. b) Timetrace of the peak wavelength for 10 different particles immersed in 20µM KCN. The green solid curve is the average of all the particles.
produces Stokes emission between roughly 630 nm and 650 nm, as observed directly on the background spectrum shown in Figure S3. This Raman band is not completely eliminated upon subtraction of the background spectrum from that of the particle. This non-additivity of the spectra indicates that water Raman scattering is significantly en-hanced by the near-field of the nanorod.
All the studied nanorods present the same qualitative behavior. Our results are sum-marized in Fig.2.3, which shows the shift of plasmon resonance wavelength as a function of time for ten different rods (dashed lines). Each nanorod shows a red shift of the plas-mon resonance wavelength which varies almost linearly with time irrespective of the initial resonance wavelength. The rate of SPR shift, however, varies significantly from particle to particle. The highest observed rate was 15 nm/minute while the lowest one was 2 nm/minute. The green curve in Figure2.3is the average of all the shifts; since spectra of each particle were acquired sequentially, we interpolated the values of the shift at intermediate times to compute the average.
The reaction between gold and potassium cyanide is well known and is used for gold mining, electroplating, etc. Gold reacts with aqueous CN−ions in presence of oxygen to
2, which is soluble in water. The reaction can be written as follows
4 Au+8 CN−+O2+2 H2O4 Au(CN)−2+4 OH−
In our experiment the formation of Au(CN)−2results in gold etching from the nanorods, as has been reported previously.
Figure 2.3: Timetrace of the peak wavelength for 10 different particles immersed in 20µM KCN. The green solid curve is the average of all the particles. The diagram shows the isotropic etching of a nanorod, leading to a higher aspect ratio.
that the one-photon-excited luminescence intensity decreases with time. Secondly, the aspect ratio of a nanorod can either decrease or increase depending on the preferred direction of etching. The Nanorod aspect ratio will decrease with time if the reaction happens preferably at the tips. This is indeed the case for nanorods protected with CTAB and dispersed in solution. CTAB binds more weakly to the tips than to the sides and therefore leaves the tips more susceptible for chemical reactions. The consequent decrease of aspect ratio yields a blue shift of the plasmon resonance. If etching happens isotropically from both sides and tips, an overall increase of the nanorod’s aspect ratio results, as is depicted schematically in Fig.2.3. This is the more likely scenario in our experiment as the nanorods’ surface does not have any protective CTAB bilayer.
Numerical simulations based on the discrete dipole approximation were performed to assess the hypothesis that the red shift of the plasmon resonance is due to isotropic nanorod etching. The initial dimensions of the particles were fixed at 25 nm×50 nm which coincide with the median values of the distribution of sizes of our nanoparticles (see SI). Simulations are carried out in etching steps of 0.5 nm. Figure2.4shows the calculated scattering spectra of the particle at different etching steps. We clearly observe a red-shift of the plasmon resonance wavelength, in concordance with what was observed in our experiment. The first inset of the figure shows the decrease of the maximum scattering cross section spectrum as a function of etched thickness.
Figure 2.4: Examples of the curves obtained at different simulations steps. The black curves are fits with Lorentzians. The left inset shows the maximum scattering cross section as function of etching. The right inset displays the plasmon shift of experimental and simulated data as the relative volume of the particle diminishes.
a given etching time would give the changes in volume and aspect ratio, which should be consistent with the same etching rate for all rods. In the present work, however, we did not attempt this analysis. We simply used the relative volume as a scaling factor to compare simulations and experiments, as is shown in the right inset of Figure2.4.
The luminescence intensity of gold nanorods is roughly proportional to their volume. It is possible therefore to calculate the relative volume of a particle by comparing the total luminescence intensity at a given instant and at a reference time. We employed the initial intensity as the reference, therefore the SPR shift increases while the relative volume decreases as depicted by the arrow in the inset of Figure2.4. The volume of the simulated particle can be directly computed from the geometrical parameters. The inset shows a remarkable agreement between the simulations and the experimental data. For smaller relative volumes (less than 0.1) the recorded spectra are 10 times less intense than the initial one, giving rise to a less accurate positioning of the resonance peak.
Figure2.5shows simulated plasmon shift rates for three different series of nanorods. In each series particles have the same initial volume, but different initial plasmon resonance, spanning from 600 nm to 780 nm. The first series corresponds to 5 particles with a volume of 6800 nm3(red), the second to 7 particles of 20000 nm3(green) and the third to 6 of 25000 nm3(blue). The shift rate is defined as the plasmon shift given by etching a thickness of 0.5 nm away from the particle. It can be observed that for larger particles the shift is slower than for smaller ones at the same initial resonance. On the other hand it is also possible to observe that red-shifted particles present a larger shift rate.
Figure 2.5: Shift rate as a function of the initial plasmon resonance for different particles. The lines correspond to particles with the same initial volume but different initial aspect ratios. As expected from an isotropic etching, larger particles will present a slower plasmon shift and more elongated particles will have a faster one.
of etching than bigger particles. This explains why smaller particles show a higher shift rate than more massive ones. On the other hand, volume is not the only factor to take into account. Particles with a higher initial aspect ratio (longer resonance wavelength) will show a faster change in aspect ratio when subjected to the same amount of etching. The interplay between both volume and initial aspect ratio can account for the big variability observed experimentally. This is also supported by the distribution of particle sizes and aspect ratios observed in the SEM images (seeA.2.)
Figure2.6shows the measured FWHM of the plasmon peak for several nanorods immersed in 20µM KCN as a function of the resonance shift. Note that the plot shows the width of the resonance in units of energy and not in units of wavelength. Because of the nonlinear relation between them, the peak width expressed in wavelength depends on the peak position rendering difficult the comparison of widths during the shift. At the beginning of the reaction there is a decrease of the width. Then it stabilizes for shifts between 75 nm and 100 nm. After this point, as the volume of the particles is largely reduced, it is no longer possible to reliably extract information from the spectra. The inset of Fig.2.6shows the FWHM obtained from the simulations for a 25 nm×50 nm nanorod. The simulated spectrum is slightly narrower than the measured one but the trends are similar.
Figure 2.6: Measured plasmon FWHM of different particles immersed in 20µM KCN as a function of their plasmon shift. The inset shows the results from the simulations carried out with the ADDA package. b) SPR Shift as a function of time for particles with the same initial SPR at different KCN concentrations.
from the particle. On the other hand we observe that the energy distance between the longitudinal plasmon peak and interband transitions in gold increases during the etching process. Therefore the non-radiative damping mechanisms in the particle may also become less efficient. Both effects combined can account for the diminishing plasmon width that is observed.
Figure2.7shows the plasmon peak shift as a function of time for various KCN concen-trations for particles with a plasmon peak at roughly 630 nm. As shown for the simulations (Figure2.5), the etching rate depends on the initial SPR, therefore it is important to choose particles that are similar to each other. The time-traces of the peak position clearly show that the shift rate is proportional to the concentration of KCN. For every concentration a shift of at least 100 nm was observed. It is important to note that the behavior of the FWHM in all the cases is similar and it resembles the results shown in Figure2.7.
Samples of the same nanorods were prepared for scanning electron microscopy (SEM) imaging by drop-casting the same solution of rods. SEM images were acquired before the etching, after 2 min immersion in KCN and after 4 min. In each case we observed that when particles are isolated from each other, the rod shape is preserved. In aggregates of particles this no longer holds and rods start to lose their shape (see Supporting Informa-tion for SEM images.) Calculating the distribuInforma-tion of sizes of the particles shows a slight increase in the aspect ratio but this shift is smaller than the width of the distribution.
Figure 2.7: SPR Shift as a function of time for particles with the same initial SPR at different KCN concentrations.
The same experiments performed in solution (see SI) show a different behavior of the plasmon resonance. As reported by other groups [22,25] the rods reshape into spheres. The presence of CTAB can explain this trend: the tips will be more exposed and therefore react more quickly, yielding a net decrease in aspect ratio. In our single-particle experiments CTAB was removed both by rinsing the samples with water and by placing them in an ozone cleaner. However, the glass surface supporting the rods has to be taken into account. In principle there is a side of the rods in contact with the surface that will be less, or not, exposed to KCN. Etching in this case wouldn’t be isotropic and would flatten the rods. Neither the optical nor the SEM images allowed us to assess this question because there is no information on the axis perpendicular to the surface. The deviation of the experiments from the simulations for the smaller volumes may be also dependent on this.
In this work we have shown a simple method that allowed us to tune the plasmon peak position of single gold nanorods with nanometer accuracy and over the range of 100 nm (300 meV). More importantly, we show that during the etching process the rod-like shape is preserved; this was confirmed both by monitoring the FWHM of the resonance peak and by acquiring SEM images after different reaction times. The experiments allowed us to record the plasmon peak with a relatively high temporal and spectral accuracy, allowing us to stop the reaction when the resonance is at the desired value.
simulations. Combining these results provides a way of predicting the behaviour of the plasmon peak for different rods.
We observed a broad distribution of the rate at which the plasmon peak shifts for different particles under the same experimental conditions. This can be attributed to the initial differences in aspect ratios and volumes of each particle. Sphere-like particles will show a small shift since the aspect ratio remains constant under isotropic etching. More elongated particles, on the other hand, will have a much steeper increase in aspect ratio while being etched. Intrinsic differences between particles can also be present, producing different shift rates even if particles have the same plasmon resonance. For instance the faceting of the surface or the prescence of left-over CTAB that was not completely washed away or oxidized can induce a slightly anisotropic etching. These differences between particles are impossible to assess by optical means and would require a much more sensitive approach.
The role of the capping agent has largely been studied and has always been held responsible for the observations both in chemical etching and for photothermal reshaping. Avoiding the presence of the passivating layers is impossible in suspension, since gold nanoparticles would aggregate. Our results provide evidence that supports previous observations regarding the effect of the curvature and the accessibility of KCN to the surface of the particle.
 C. Sönnichsen, T. Franzl, T. Wilk, G. von Plessen, J. Feldmann, O. Wilson, and P. Mulvaney,Drastic Reduction of Plasmon Damping in Gold Nanorods,Phys. Rev. Lett.88, 077402 (2002).
 M. Yorulmaz, S. Khatua, P. Zijlstra, A. Gaiduk, and M. Orrit,Luminescence quantum yield of single gold nanorods.Nano Lett.12, 4385 (2012).
 P. Zijlstra, P. M. R. Paulo, and M. Orrit,Optical detection of single non-absorbing molecules using the surface plasmon resonance of a gold nanorod.Nat. Nanotechnol.
7, 379 (2012).
 S. T. Sivapalan, B. M. Devetter, T. K. Yang, T. van Dijk, M. V. Schulmerich, P. S. Carney, R. Bhargava, and C. J. Murphy,Off-resonance surface-enhanced Raman spectroscopy from gold nanorod suspensions as a function of aspect ratio: not what we thought.
ACS Nano7, 2099 (2013).
 T. Zhao, K. Yu, L. Li, T. Zhang, Z. Guan, N. Gao, P. Yuan, S. Li, S. Q. Yao, Q.-H. Xu, and G. Q. Xu,Gold nanorod enhanced two-photon excitation fluorescence of pho-tosensitizers for two-photon imaging and photodynamic therapy.ACS Appl. Mater. Interfaces6, 2700 (2014).
 P. Zijlstra and M. Orrit,Single metal nanoparticles: optical detection, spectroscopy and applications,Reports Prog. Phys.74, 106401 (2011).
 S. Khatua, P. M. R. Paulo, H. Yuan, A. Gupta, P. Zijlstra, and M. Orrit,Resonant plasmonic enhancement of single-molecule fluorescence by individual gold nanorods.